Materials of all types are often heat treated to im- prove their properties. The phenomena that occur during a heat treatment almost always involve atomic diffusion. Often an enhancement of diffusion rate is desired; on occasion measures are taken to reduce it. Heat-treating temperatures and times, and/or cooling rates are often predictable using the
mathematics of diffusion and appropriate diffusion constants. The steel gear shown on this page has been case hardened (Section 9.14); that is, its hard- ness and resistance to failure by fatigue have been enhanced by diffusing excess carbon or nitrogen into the outer surface layer.
L e a r n i n g O b j e c t i v e s
After studying this chapter you should be able to do the following: 1. Name and describe the two atomic mechanisms
2. Distinguish between steady-state and nonsteady- state diffusion.
3. (a) Write Fick’s first and second laws in equa- tion form, and define all parameters. (b) Note the kind of diffusion for which each of
these equations is normally applied.
Many reactions and processes that are important in the treatment of materials rely on the transfer of mass either within a specific solid (ordinarily on a microscopic level) or from a liquid, a gas, or another solid phase. This is necessarily accomplished by diffusion, the phenomenon of material transport by atomic motion. This chapter discusses the atomic mechanisms by which diffusion occurs, the mathematics of diffusion, and the influence of temperature and diffusing species on the rate of dif- fusion.
The phenomenon of diffusion may be demonstrated with the use of a diffusion
couple, which is formed by joining bars of two different metals together so that
there is intimate contact between the two faces; this is illustrated for copper and nickel in Figure 6.1, which includes schematic representations of atom positions and composition across the interface. This couple is heated for an extended period at an elevated temperature (but below the melting temperature of both metals), and cooled to room temperature. Chemical analysis will reveal a condition similar to that represented in Figure 6.2, namely, pure copper and nickel at the two extremit- ies of the couple, separated by an alloyed region. Concentrations of both metals vary with position as shown in Figure 6.2c. This result indicates that copper atoms have migrated or diffused into the nickel, and that nickel has diffused into copper. This process, whereby atoms of one metal diffuse into another, is termed interdiffu-
sion, or impurity diffusion.
Interdiffusion may be discerned from a macroscopic perspective by changes in concentration which occur over time, as in the example for the Cu–Ni diffusion couple. There is a net drift or transport of atoms from high to low concentration regions. Diffusion also occurs for pure metals, but all atoms exchanging positions are of the same type; this is termed self-diffusion. Of course, self-diffusion is not normally subject to observation by noting compositional changes.
From an atomic perspective, diffusion is just the stepwise migration of atoms from lattice site to lattice site. In fact, the atoms in solid materials are in constant motion, rapidly changing positions. For an atom to make such a move, two conditions must be met: (1) there must be an empty adjacent site, and (2) the atom must have sufficient energy to break bonds with its neighbor atoms and then cause some lattice distortion during the displacement. This energy is vibrational in nature (Section 5.10). At a specific temperature some small fraction of the total number of atoms
4. Write the solution to Fick’s second law for diffu- sion into a semi-infinite solid when the concen- tration of diffusing species at the surface is held constant. Define all parameters in this equation. 5. Calculate the diffusion coefficient for some mate-
rial at a specified temperature, given the appro- priate diffusion constants.
6. Note one difference in diffusion mechanisms for metals and ionic solids.
128 ● Chapter 6 / Diffusion Cu Ni Cu Ni 100 0 Concentration of Ni, Cu (a ) ( b) (c ) Position
FIGURE6.1 (a) A copper–nickel diffusion couple
before a high-temperature heat treatment. (b) Schematic representations of Cu (colored circles) and Ni (gray circles) atom locations within the diffusion couple. (c) Concentrations of copper and nickel as a function of position across the couple.
FIGURE6.2 (a) A copper–nickel diffusion couple
after a high-temperature heat treatment, showing the alloyed diffusion zone. (b) Schematic representations of Cu (colored circles) and Ni (gray circles) atom locations within the couple. (c) Concentrations of copper and nickel as a function of position across the couple. Concentration of Ni, Cu Position Ni Cu 0 100 (c) (b) (a) Diffusion of Ni atoms Diffusion of Cu atoms Cu-Ni alloy Ni Cu
6.2 Diffusion Mechanisms ● 129
is capable of diffusive motion, by virtue of the magnitudes of their vibrational energies. This fraction increases with rising temperature.
Several different models for this atomic motion have been proposed; of these possibilities, two dominate for metallic diffusion.